LMucko/crystallography-open-database huggingface dataset:
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 400 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007212
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1316
_cell_length_b                   8.1316
_cell_length_c                   8.1316
_cell_formula_units_Z            8
_cell_volume                     537.685
_database_code_amcsd             0008797
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.623
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007212
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 450 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007213
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 450 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1354
_cell_length_b                   8.1354
_cell_length_c                   8.1354
_cell_formula_units_Z            8
_cell_volume                     538.439
_database_code_amcsd             0008798
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    3.618
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007213
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 400 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007214
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1315
_cell_length_b                   8.1315
_cell_length_c                   8.1315
_cell_formula_units_Z            8
_cell_volume                     537.665
_database_code_amcsd             0008799
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.623
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007214
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 25 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007215
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1085
_cell_length_b                   8.1085
_cell_length_c                   8.1085
_cell_formula_units_Z            8
_cell_volume                     533.116
_database_code_amcsd             0008800
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.654
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007215
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 2nd run, T = 500 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007216
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 2nd run, T = 500 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1400
_cell_length_b                   8.1400
_cell_length_c                   8.1400
_cell_formula_units_Z            8
_cell_volume                     539.353
_database_code_amcsd             0008801
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.612
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007216
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 2nd run, T = 450 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007217
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 2nd run, T = 450 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1358
_cell_length_b                   8.1358
_cell_length_c                   8.1358
_cell_formula_units_Z            8
_cell_volume                     538.519
_database_code_amcsd             0008802
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    3.618
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007217
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 550 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007218
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 550 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1445
_cell_length_b                   8.1445
_cell_length_c                   8.1445
_cell_formula_units_Z            8
_cell_volume                     540.248
_database_code_amcsd             0008803
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    3.606
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007218
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 600 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007219
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1482
_cell_length_b                   8.1482
_cell_length_c                   8.1482
_cell_formula_units_Z            8
_cell_volume                     540.985
_database_code_amcsd             0008804
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.601
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007219
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 650 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007220
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 650 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1525
_cell_length_b                   8.1525
_cell_length_c                   8.1525
_cell_formula_units_Z            8
_cell_volume                     541.842
_database_code_amcsd             0008805
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    3.596
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007220
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 700 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007221
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1569
_cell_length_b                   8.1569
_cell_length_c                   8.1569
_cell_formula_units_Z            8
_cell_volume                     542.719
_database_code_amcsd             0008806
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.590
_cod_original_cell_volume        542.720
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007221
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 800 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007222
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1655
_cell_length_b                   8.1655
_cell_length_c                   8.1655
_cell_formula_units_Z            8
_cell_volume                     544.438
_database_code_amcsd             0008807
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.578
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007222
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 900 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007223
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 900 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1726
_cell_length_b                   8.1726
_cell_length_c                   8.1726
_cell_formula_units_Z            8
_cell_volume                     545.859
_database_code_amcsd             0008808
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.569
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007223
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 3rd run, T = 1000 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007224
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 3rd run, T = 1000 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1791
_cell_length_b                   8.1791
_cell_length_c                   8.1791
_cell_formula_units_Z            8
_cell_volume                     547.163
_database_code_amcsd             0008809
_diffrn_ambient_temperature      1273.15
_exptl_crystal_density_diffrn    3.561
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007224
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: L-Fe, 1st run, T = 25 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007225
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: L-Fe, 1st run, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.914 Fe0.082 Mg0.99 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0989
_cell_length_b                   8.0989
_cell_length_c                   8.0989
_cell_formula_units_Z            8
_cell_volume                     531.225
_database_code_amcsd             0008810
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.608
_cod_original_cell_volume        531.224
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.914 Fe.082 Mg.99 O4'
_cod_database_code               9007225
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: L-Fe, 1st run, T = 200 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007226
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: L-Fe, 1st run, T = 200 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.917 Fe0.081 Mg0.988 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1092
_cell_length_b                   8.1092
_cell_length_c                   8.1092
_cell_formula_units_Z            8
_cell_volume                     533.254
_database_code_amcsd             0008811
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    3.594
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.917 Fe.081 Mg.988 O4'
_cod_database_code               9007226